**ANNALS OF THE UNIVERSITY OF ORADEA **
**FASCICLE OF TEXTILES, LEATHERWORK**

**THE OPTIMIZATION OF PLUSH YARNS BULKING PROCESS **

**VINEREANU Adam1, POTOP Georgeta-Lidia2, LEON Ana-Lacramioara2, **
**VINEREANU Elena1**

*1*

*Technical College “Ion I.C. Bratianu”, Plazza Iancu Huniade no. 2, *
*300002-Timisoara, ROMANIA, E-Mail: elenavinereanu@yahoo.com *

*2*

* Technical University “Gh. Asachi” of Iasi, Faculty of Textiles, Leather Goods & Industrial Management, *
*Department of Engineering & Design of Textile Products, Bd. D. Mangeron no. 29, 700050-Iasi, ROMANIA, *

*E-Mail: gpotop@tex.tuiasi.ro*, *ana_leon@yahoo.com *

Corresponding author: Leon Ana-Lacramioara, E-mail: ana_leon@yahoo.com

**Abstract: This paper presents the experiments that were conducted on the installation of continuous bulking and ***thermofixing “SUPERBA” type TVP-2S for optimization of the plush yarns bulking process. There were *
*considered plush yarns Nm 6.5/2, made of the fibrous blend of 50% indigenous wool sort 41 and 50% PES. In *
*the first stage, it performs a thermal treatment with a turboprevaporizer at a temperature lower than *
*thermofixing temperature, at atmospheric pressure, such that the plush yarns - deposed in a freely state on a belt *
*conveyor - are uniformly bulking and contracting. *

*It was followed the mathematical modeling procedure, working with a factorial program, rotatable central *
*composite type, and two independent variables. After analyzing the parameters that have a direct influence on *
*the bulking degree, there were selected the pre-vaporization temperature (coded x1,oC) and the velocity of belt *
*inside pre-vaporizer (coded x2, m/min). As for the dependent variable, it was chosen the plush yarn diameter *
*(coded y, mm). There were found the coordinates of the optimal point, and then this pair of values was verified in *
*practice. These coordinates are: x1optim = 90oC and x2optim = 6.5 m/min. The conclusion is that the goal was *
*accomplished: it was obtained a good cover degree for double-plush carpets by reducing the number of tufts per *
*unit surface. *

* Key words: woollen carpet, double plush technology, mathematical model, yarn diameter*.

**1. INTRODUCTION **

Using modern technologies and performing equipment to obtain qualitatively plush carpets

*with reduced manufacturing costs* represents a priority for any trading company that has as object of

activity to produce and trade carpets.

The real value of a carpet is determined by its physical and mechanical properties: carpet mass and thickness; behaviour in static and dynamic regime; resistance to friction wear; resistance to tufts pulling; charging with static electricity; soiling sensitivity; capacity of thermal and phonic insulation [1]

By analyzing the advantages and disadvantages of manufacturing technologies for mechanically woven carpets, one can conclude that double-plush weaving technology is recommended when wishing to satisfy higher and higher customers’ demands from the standpoint of comfort and other utilization characteristics offered by carpet.

**2. MATERIALS AND METHOD **

The installation of continuous bulking and thermofixing “SUPERBA” performs, in the first stage, a thermal treatment by means of a thermo-vaporizer at a temperature lower than the thermofixing temperature and at atmospheric pressure, such that the yarns freely deposed on a belt conveyor are uniformly bulking and contracting.

The main parameters that can be adjusted at this installation and have a direct influence upon the bulking degree are:

- moving velocity of woollen yarns layer (v1= 0- 750 m/min); - belt conveyor velocity inside pre-vaporizer (v2= 5.5-8.6 m/min); - pre-vaporization temperature (t1 = 90-990C);

- vapor temperature in the thermofixing tunnel (99.1- 150.240C).

There were chosen as independent variables: x1- pre-vaporization temperature (0C) and x2 – velocity of belt conveyor in pre-vaporizer (m/min) because previous researches showed that they have the greatest influence on bulking process of plush yarns. The dependent variable y (mm) is the diameter of the plush yarn Nm 6.5/2, obtained from the fibrous blend 50% indigenous wool sort 41and 50% PES.

We have used the factorial program, *rotatable central composite type*, with two variables at
five variation levels (-1.414, -1, 0, 1, +1.414). It was used the central composite designbecause it is
very efficient and provides much information in a minimum number of required runs. The existence of
five central points (x1=0, x2=0) helps the researcher to improve the precision of the experiments. A
design is called “rotatable” if the variance of the estimated response depends on the distance from the
centre of the design.

The experiments were carried out according to an experiment matrix (Table 1) for two independent variables. Mathematical modeling was used to optimize the plush yarn bulking process [4,5,6]. The general form of the 2-variables second order regression equation is:

*y = b0 + b1 x1 + b2 x2 + b11 x12 +b22 x22 + b12 x1x2 + ε* **(1)**

It was determined the second order regression equation based on the matrix of experiments:

*y = 0.726975 + 0.002091 x1 -0.00096 x2 -0.0014 x12 +0.00015 x22 – 0.0005 x1x2* **(2) **

**Table 1.**Matrix of experiments

Independent variables Dependent variable

x1

(0C)

x2

(m/min) No.

code real code real

ymas
(mm)
ycalc
(mm)
∆_{y }
(%)

1 -1 92 -1 6 0.725 0.72379094 0.17

2 1 94 -1 6 0.728 0.72897244 -0.13

3 -1 92 1 6.5 0.725 0.72287694 0.29

4 1 94 1 6.5 0.726 0.72605844 -0.08

5 -1.414 90 0 7 0.717 0.72121859 -0.59

6 1.414 96 0 7 0.726 0.72713123 -0.16

7 0 95 -1.414 5.5 0.726 0.7280286 -0.28

8 0 95 1.414 8 0.722 0.7253222 -0.46

9 0 95 0 7 0.726 0.72697462 -0.13

10 0 95 0 7 0.728 0.72697462 0.14

11 0 95 0 7 0.726 0.72697462 -0.13

12 0 95 0 7 0.726 0.72697462 -0.13

**ANNALS OF THE UNIVERSITY OF ORADEA **
**FASCICLE OF TEXTILES, LEATHERWORK**

In the last column of Table 1 there are written the values of ∆_{y , computed with the following }
formula:
100
y
y
y
y
mas
calc
mas
⋅
−
=

∆ (%) **(3)**

The value ∆_{y shows the difference between the measured value of yarn diameter (coded ymas) }
and the computer value of diameter (coded ycalc). It is noticed that ∆_{y can be positive or negative. }

The significance of the coefficients for the regression equation (2) was tested by the Student test, accordingly to the Table 2.

**Table 2.**Significance test for the coefficients of the regression equation

** **

The critical value for Student test was taken from a table: tα;ν = t0.05; 6 = 1.94.

The model adequacy was verified by means of the Fisher-Snedecor test and with percentage deviations. The computed value Fc = 3.27 is higher than the critical value taken from the table Fν1,ν2,α = F12;12;0.05 = 2.69.

The mathematical model conformity degree was verified by the same test. The computed value Fc is 11.47, which means that it is smaller than the critical table value Ftab = Fν1,ν2,α = 15.98.

Also the Fisher-Snedecor test was used to verify the deviation of the sampling data from the mean (average) value. The computed value Fc = 21.82 is higher than the critical value from the table, Ftab = F0.05;12.4 = 5.91 which indicates that the deviations are due to the independent variables and not to some experimental errors [5].

In the end, it was computed the correlation coefficient r ymas;ycalc = 0.79123 by *Microsoft Excel *

application. This value shows a pretty good agreement between the experimental and predicted values from the model.

From the analysis of the equation coefficients, there can be formulated the following conclusions:

• The sign (+) for the coefficient b1 and the sign (–) for the coefficient b2 show that the two independent parameters have a different influence on the resultative variable y, i.e. the increase of yarn diameter is more significant when the temperature increases and the yarn velocity through the vaporizer decreases.

• The ratio between the coefficients of the quadratic terms and the free term indicates a variation rate of the yarn diameter of 0.19% due to temperature modification, and of 0.02% due to the modification of the standing time in the pre-vaporization zone.

The response surface of the regression equation has a parabolic shape like a bowl that opens downward (shown in Figure 1). Its maximum has the coordinates: x1 = -1.41 and x2 = 1, corresponding to the pair of natural values:

x1optim = 900C x2optim = 6.5 m/min.

Figure 2 puts in evidence the influence exerted by x1 and x2 that act simultaneously upon y. Figures 3 and 4 show the influences of these two working parameters that act independently on the plush yarn diameter.

ti Coefficients of regression equation

tc0 3029061 b0 significant

tc1 13938.33 b1 significant

tc2 -6380 b2 significant

tc11 -8114.71 b11 significant

tc22 -8672.46 b22 significant

**Fig. 2: Influence of temperature (x1) and belt velocity through the pre- vaporizer (x2) ***on the plush yarn diameter *

**ANNALS OF THE UNIVERSITY OF ORADEA **
**FASCICLE OF TEXTILES, LEATHERWORK**

**Fig: 4. Influence of belt velocity through the pre-vaporizer (x2) *** on theplush yarn diameter *

From the previous graphics, one can notice that the optimum values of the yarn diameter increase through the pre-vaporizer are obtained for the pair of coded values: x1 = -1.414 and x2= 1, and x1 = 0, x2= 1.414 respectively, corresponding to the pair of natural values:

- x1 = 900C and x2 = 6.5 m/min; - x2 = 950C and x2 = 8 m/min.

Since the value of the parameter x2 = 8m/min is close to the maximum admissible working speed of pre-vaporizing and thermofixing installation, we recommend the utilization of the pairs of values: x1= 900C and x2= 6.5 m/min, which provides the optimum value for theresultative, as well as a reduced power intake.

Then we proceeded to the verification of optimal values. With this aim in view, we made temperature and velocity adjustments resulted from optimization, and the measured value of the yarn diameter was of 0.749. The computed value of 0.726 represents an increase by 3.2%, which leads to the conclusion that the process optimization according to the mathematical model was accomplished.

**3. CONCLUSIONS **

The goal of this research was to accomplish an optimal cover degree for double-plush carpets by reducing the number of tufts per unit surface.

This paper presents a bulking method for the plush yarns Nm 6.5/2, obtained from the fibrous blend 50% indigenous wool sort 41 and 50% PES.

Experiment planning carried out on the installation of continuous bulking and thermofixing “SUPERBA” was based on the matrix specific to the factorial program, rotatable central composite type, with two variables at five levels of variation. After mathematical modeling procedure, it was found the optimum point with the coordinates (in natural values): pre-vaporizing temperature of 900C (coded x1) and belt velocity in pre-vaporizer of 6.5 m/min (coded x2).

“Gheorghe Asachi” din Iasi, 2010.

[2] C. Vilcu, G.L. Potop, “*Double plush carpets based on chemically modified *

*polypropylene*”, Bul. IPI Iasi, Tomul LVI (LX), fasc. 1, Sectia Textile-Pielarie, 2010, pp. 87-92.

[3] A. Bucevschi, A. Popa, M. Gheorghiu, *“Studiul influentei caracteristicilor firelor asupra *

*caracteristicilor tesaturilor”, * Sesiunea de comunicari stiintifice, Universitatea ”Aurel Vlaicu”,

Arad,1996.

[4] M. Ciocoiu,*“Pachete de programe pentru modelarea matematica a proceselor textile”, *

Lito, Iasi, 1996.

[5] M. Ciocoiu, *“Prelucrarea statistico-matematica a datelor experimentale”*, Editura
Performantica, Iasi, 2002.

[6] L. Cioara, O. Marchis, I. Cioara, *“Optimizarea structurii tesute, sursa de efecte economice *